title: ÐÐ»Ð¸ÑÐ¸ÑÐ¾Ð²Ð°Ð½Ð¸Ðµ Ð¼Ð½Ð¾Ð³Ð¾ÐºÐ¾Ð¼Ð¿Ð¾Ð½ÐµÐ½ÑÐ½ÑÑ ÑÐ¿Ð»Ð°Ð²Ð¾Ð² Ð½Ð° Ð¾ÑÐ½Ð¾Ð²Ðµ ÑÐ¸ÑÑÐµÐ¼Ñ FeNiCr
title: Ð²ÑÐ¿ÑÑÐºÐ½Ð°Ñ ÐºÐ²Ð°Ð»Ð¸ÑÐ¸ÐºÐ°ÑÐ¸Ð¾Ð½Ð½Ð°Ñ ÑÐ°Ð±Ð¾ÑÐ° Ð¼Ð°Ð³Ð¸ÑÑÑÐ°
titleType: Subtitle
title: Alliteration of multicomponent alloys based on the FeNiCr system
Creators: name: ÐÑÐ´ÑÐ°Ð²ÐµÑ, ÐÐ»Ð¸Ð·Ð°Ð²ÐµÑÐ°
Publisher: name: Ð¡Ð°Ð½ÐºÑ-ÐÐµÑÐµÑÐ±ÑÑÐ³ÑÐºÐ¸Ð¹ Ð¿Ð¾Ð»Ð¸ÑÐµÑÐ½Ð¸ÑÐµÑÐºÐ¸Ð¹ ÑÐ½Ð¸Ð²ÐµÑÑÐ¸ÑÐµÑ ÐÐµÑÑÐ° ÐÐµÐ»Ð¸ÐºÐ¾Ð³Ð¾
Year: 2023
Subjects: Ð°Ð»Ð¸ÑÐ¸ÑÐ¾Ð²Ð°Ð½Ð¸Ðµ
Ð¸Ð½ÐºÐ¾Ð½ÐµÐ»Ñ
Ð¿Ð¾ÐºÑÑÑÐ¸Ðµ
Ð²ÑÑÐ¾ÐºÐ¾ÑÐ½ÑÑÐ¾Ð¿Ð¸Ð¹Ð½ÑÐ¹ ÑÐ¿Ð»Ð°Ð²
ÑÐ°Ð·Ð¾Ð²ÑÐ¹ ÑÐ¾ÑÑÐ°Ð²
alitation
inconel
coating
high entropy alloy
phase composition

description: ÐÐ°Ð½Ð½Ð°Ñ ÑÐ°Ð±Ð¾ÑÐ° Ð¿Ð¾ÑÐ²ÑÑÐµÐ½Ð° Ð¸ÑÑÐ»ÐµÐ´Ð¾Ð²Ð°Ð½Ð¸Ñ Ð¿Ð¾ÐºÑÑÑÐ¸Ð¹ Ð½Ð° Incoloy 825 Ð¸ Ð²ÑÑÐ¾ÐºÐ¾ÑÐ½ÑÑÐ¾Ð¿Ð¸Ð¹Ð½ÑÐ¹ ÑÐ¿Ð»Ð°Ð² FeNiCoCrMo0,5 Ð¿Ð¾Ð»ÑÑÐµÐ½Ð½ÑÐµ Ð¿ÑÐ¸ Ð¿Ð¾ÑÐ¾ÑÐºÐ¾Ð²Ð¾Ð¼ Ð°Ð»Ð¸ÑÐ¸ÑÐ¾Ð²Ð°Ð½Ð¸Ð¸. ÐÐ°Ð´Ð°ÑÐ¸, ÐºÐ¾ÑÐ¾ÑÑÐµ ÑÐµÑÐ°Ð»Ð¸ÑÑ Ð² ÑÐ¾Ð´Ðµ Ð¸ÑÑÐ»ÐµÐ´Ð¾Ð²Ð°Ð½Ð¸Ñ: 1. ÐÑÐ¾Ð¸Ð·Ð²ÐµÑÑÐ¸ Ð¿Ð¾ÐºÑÑÑÐ¸Ðµ Ð½Ð° Ð¾Ð±ÑÐ°Ð·ÑÑ Ð¿ÑÐ¸ Ð¸Ð·Ð¼ÐµÐ½ÐµÐ½Ð¸Ð¸ Ð¾Ð±ÑÐ°Ð·ÑÐ¾Ð² Ð¸ ÑÐµÐ¼Ð¿ÐµÑÐ°ÑÑÑÑ. 2. ÐÐ¿ÑÐµÐ´ÐµÐ»Ð¸ÑÑ Ð²Ð»Ð¸ÑÐ½Ð¸Ðµ ÑÐ°Ð·Ð»Ð¸ÑÐ½ÑÑ Ð¿Ð°ÑÐ°Ð¼ÐµÑÑÐ¾Ð² Ð½Ð° ÑÑÑÑÐºÑÑÑÑ Ð¸ ÑÐ²Ð¾Ð¹ÑÑÐ²Ð° Ð¿Ð¾Ð»ÑÑÐ°ÐµÐ¼ÑÑ Ð¼Ð°ÑÐµÑÐ¸Ð°Ð»Ð¾Ð². Ð ÑÐ°Ð±Ð¾ÑÐµ Ð±ÑÐ»Ð¸ Ð¿ÑÐ¾Ð²ÐµÐ´ÐµÐ½Ñ Ð¸ÑÑÐ»ÐµÐ´Ð¾Ð²Ð°Ð½Ð¸Ñ Ð¸ ÑÐ°ÑÑÑÑÑ, Ð¿Ð¾ÐºÐ°Ð·ÑÐ²Ð°ÑÑÐ¸Ðµ Ð½Ð° Ð¼Ð¸ÐºÑÐ¾ÑÑÑÑÐºÑÑÑÑ Ð¸ ÑÐ²Ð¾Ð¹ÑÑÐ²Ð° Ð¿Ð¾ÐºÑÑÑÐ¸Ð¹. ÐÐ½Ð°Ð»Ð¸Ð· Ð¿ÑÐ¾Ð²Ð¾Ð´Ð¸Ð»ÑÑ Ñ Ð¿Ð¾Ð¼Ð¾ÑÑÑ SEM, ÑÐµÐ½ÑÐ³ÐµÐ½Ð¾ÑÑÑÑÐºÑÑÑÐ½Ð¾Ð³Ð¾ Ð°Ð½Ð°Ð»Ð¸Ð·Ð°. Ð ÑÐµÐ·ÑÐ»ÑÑÐ°ÑÐµ ÑÐ°Ð±Ð¾ÑÑ Ð±ÑÐ»Ð¸ Ð¿ÑÐ¾Ð°Ð½Ð°Ð»Ð¸Ð·Ð¸ÑÐ¾Ð²Ð°Ð½Ñ ÑÐ°Ð·Ð¼ÐµÑÑ Ð¿Ð¾Ð»ÑÑÐµÐ½Ð½ÑÑ Ð¿Ð¾ÐºÑÑÑÐ¸Ð¹ Ð¿ÑÐ¸ ÑÐ°Ð·Ð½ÑÑ ÑÐµÐ¼Ð¿ÐµÑÐ°ÑÑÑÐ°Ñ Ð¸ Ð¸Ñ ÑÐ°Ð·Ð¾Ð²ÑÐµ ÑÐ¾ÑÑÐ°Ð²Ñ Ð´Ð¾ Ð¸ Ð¿Ð¾ÑÐ»Ðµ ÑÐµÑÐ¼Ð¾Ð¾Ð±ÑÐ°Ð±Ð¾ÑÐºÐ¸. ÐÑÐ¸ ÑÐ°ÑÑÐ¼Ð¾ÑÑÐµÐ½Ð¸Ð¸ Incoloy Ð¸ Ð²ÑÑÐ¾ÐºÐ¾ÑÐ½ÑÑÐ¾Ð¿Ð¸Ð¹Ð½Ð¾Ð³Ð¾ ÑÐ¿Ð»Ð°Ð²Ð° Ð±ÑÐ»Ð¾ Ð²ÑÑÐ²Ð»ÐµÐ½Ð¾, ÑÑÐ¾ Ð¿Ð¾ÐºÑÑÑÐ¸Ðµ Ð½Ð° ÐÐ­Ð¡ Ð¿ÑÐ¸ 800Â°C Ð¸Ð¼ÐµÐµÑ ÑÐ°Ð¼ÑÑ Ð±Ð¾Ð»ÑÑÑÑ Ð¼Ð¸ÐºÑÐ¾ÑÐ²ÐµÑÐ´Ð¾ÑÑÑ Ð¾ÐºÐ¾Ð»Ð¾ 754Â±20HV, Ð° ÐµÐ³Ð¾ ÑÐ¾Ð»ÑÐ¸Ð½Ð° Ð´Ð¾ÑÑÐ¸Ð³Ð°ÐµÑ 50Â±5Ð¼ÐºÐ¼, Ð¿Ð¾ ÑÑÐ°Ð²Ð½ÐµÐ½Ð¸Ñ Ñ Ð´ÑÑÐ³Ð¸Ð¼Ð¸ Ð¾Ð±ÑÐ°Ð·ÑÐ°Ð¼Ð¸. ÐÐ´Ð½Ð°ÐºÐ¾, Ð±Ð»Ð¸Ð¶Ðµ Ðº Ð¿Ð¾Ð²ÐµÑÑÐ½Ð¾ÑÑÐ¸ ÑÐ²ÐµÑÐ´Ð¾ÑÑÑ Ð´Ð°Ð½Ð½Ð¾Ð³Ð¾ Ð¾Ð±ÑÐ°Ð·ÑÐ° ÑÐ½Ð¸Ð¶Ð°ÐµÑÑÑ Ð´Ð¾ â336HV, Ð² ÑÐ¾ Ð²ÑÐµÐ¼Ñ ÐºÐ°Ðº Ñ Incoloy 825 ÑÐ²ÐµÑÐ´Ð¾ÑÑÑ Ð¾Ñ Ð¿Ð¾Ð²ÐµÑÑÐ½Ð¾ÑÑÐ¸ Ð¸Ð·Ð¼ÐµÐ½ÑÐµÑÑÑ Ð¾Ñ 544HV Ð´Ð¾ 706HV. ÐÐ¾Ð²ÐµÑÑÐ½Ð¾ÑÑÑ Ð¾Ð±ÑÐ°Ð·ÑÐ° Incoloy 825 Ð¿ÑÐ¸ 800Â°C Ð½Ðµ ÑÐ°Ð·ÑÑÑÐ°Ð»Ð°ÑÑ Ð¿ÑÐ¸ Ð¸Ð½Ð´ÐµÐ½ÑÐ¸ÑÐ¾Ð²Ð°Ð½Ð¸Ð¸ Ð¿Ð¾ ÑÑÐ°Ð²Ð½ÐµÐ½Ð¸Ñ Ñ Ð´ÑÑÐ³Ð¸Ð¼Ð¸ Ð¾Ð±ÑÐ°Ð·ÑÐ°Ð¼Ð¸ Ð¸ ÐµÐ³Ð¾ Ð¿Ð¾ÐºÑÑÑÐ¸Ðµ Ð´Ð¾ÑÑÐ¸Ð³Ð°ÐµÑ 40Â±5Ð¼ÐºÐ¼. Ð¡Ð°Ð¼Ð¾Ðµ Ð¼Ð°Ð»ÐµÐ½ÑÐºÐ¾Ðµ Ð¿Ð¾ÐºÑÑÑÐ¸Ðµ Ð±ÑÐ»Ð¾ Ð¿Ð¾Ð»ÑÑÐµÐ½Ð¾ Ñ Incoloy 825 Ð¿ÑÐ¸ 600Â°C Ð¸ FeNiCoCrMo0,5 Ð¿ÑÐ¸ 700Â°C Ð¾Ð½Ð¾ Ð¼ÐµÐ½ÐµÐµ 5Ð¼ÐºÐ¼.
description: This work is devoted to the study of coatings on Incoloy 825 and highentropic alloy FeNiCoCrMo0,5 obtained by powder alitization. The tasks that were solved in the course of the study were: 1. To produce coating on the samples by changing samples and temperature. 2. to determine the influence of various parameters on the structure and properties of the obtained materials. In this work, studies and calculations showing on the microstructure and properties of the coatings were carried out. The analysis was carried out using SEM, X-ray structural analysis. As a result of the work, the dimensions of the obtained coatings at different temperatures and their phase compositions before and after heat treatment were analyzed. When considering Incoloy and high entropy alloy, it was found that the coating on VES at 800Â°C has the highest microhardness of about 754Â±20HV, and its thickness reaches 50Â±5Î¼m, compared to other samples. However, closer to the surface, the hardness of this sample decreases to â336HV, while Incoloy 825s hardness from the surface changes from 544HV to 706HV. The surface of Incoloy 825 sample at 800Â°C did not degrade during indentation compared to other samples and its coating reaches 40Â±5Î¼m. The smallest coating was obtained for Incoloy 825 at 600 Â° C and FeNiCoCrMo0.5 at 700Â°C was less than 5Âµm.